Journal of Advanced Research (2013) 4, 61–67
Journal of Advanced Research
Eﬀect of endodontic irrigation and dressing procedures on the shear bond strength of composite to coronal dentin Sahar E. Abo-Hamar
University of Tanta, Faculty of Dentistry, Department of Dental Materials, El-Geish Street, 31111 Tanta, Egypt Received 11 October 2011; revised 18 January 2012; accepted 18 January 2012 Available online 3 March 2012
KEYWORDS Bond strength to coronal dentin; NaOCl; Glyde-File-Prep; Ca(OH)2
Abstract This study aimed to evaluate the effects of three sodium hypochlorite (NaOCl)-endodontic irrigation procedures used alone or in combinations with two intermediate dressing materials on bond strengths of two adhesive composite systems to coronal dentin. Surfaces were treated with NaOCl or NaOCl–Glyde-File-Prep (H2O2 and EDTA) with or without chlorhexidine (CHX) as a ﬁnal rinse. Intermediate dressing materials of calcium hydroxide (Ca(OH)2) and sodium perborate (SP) were combined with surface treatments. Surface treatment groups (n = 10/group) included (1) distilled water (control), (2) 5.25% NaOCl (30 min), (3) NaOCl/Glyde (30 min), (4) NaOCl/Glyde (30 min) + CHX (2 min), (5) NaOCl/Glyde (30 min) + Ca(OH)2 (5 days) + CHX (2 min), and (6) NaOCl/Glyde (30 min) + SP (9 days) + CHX (2 min). For each surface treatment group, dentin shear bond strengths of two different composite systems (Excite/Tetric Flow Chroma, [EX/TFC], and Clearﬁl Protect Bond/Protect Liner F [PB/PLF]) were evaluated. Median shear bond strengths (EX/TFC, PB/PLF) for each surface treatment group in MPa were (1) 21, 18; (2) 26, 18; (3) 21, 17; (4) 22, 16; (5) 17, 11; and (6) 14, 11, respectively. NaOCl signiﬁcantly increased the bond strength of EX/TFC (p < 0.05), but did not signiﬁcantly affect that of PB/PLF. The use of NaOCl/Glyde with CHX did not signiﬁcantly affect EX/TFC (p > 0.05), whereas it signiﬁcantly decreased PB/PLF (p < 0.05). Ca(OH)2 and SP signiﬁcantly decreased the bond strengths of both adhesive systems (p < 0.05). Adhesion to coronal dentin is dependent upon the irrigation regimen and the type of adhesive. ª 2012 Cairo University. Production and hosting by Elsevier B.V. All rights reserved.
* Tel.: +20 40 3345314, +20 104975569 (mobile); fax: +20 40 3330320. E-mail address: [email protected]
2090-1232 ª 2012 Cairo University. Production and hosting by Elsevier B.V. All rights reserved. Peer review under responsibility of Cairo University. doi:10.1016/j.jare.2012.01.004
Production and hosting by Elsevier
62 Introduction One of the primary goals of root canal treatment is to eliminate bacteria from the root canal system, which have been shown to be the etiology for apical periodontitis and endodontic failure. Furthermore, restoring of the tooth after root canal treatment should be capable of preventing recontamination of the root canal system . The use of dentin adhesive systems and ﬂowable composite resin has been advocated for use within the pulp chamber/access cavity in an attempt to work as an oriﬁce barrier against microleakage . However, endodontic materials inevitably contact the dentin of the access cavity during chemomechanical root canal preparation, therefore the dentin available for the coronal restoration may be modiﬁed and bonding procedures may also be affected [3–8]. Sodium hypochlorite (NaOCL) (5.25%) has been highly recommended as root canal irrigant due to its antibacterial and organic tissue dissolution properties . However, it has been reported that it induces oxidations of some components in the dentin matrix [4,5] and also causes dentin subsurface deproteinization . In literature, NaOCl irrigant was found to decrease the bond strengths of some adhesive systems [3–6] that was recovered by using reducing agents as sodium ascorbate [4,5], whereas it did not affect [3,5,7] or even increased  the bond strengths of other adhesives to coronal dentin. The strategy of alternating irrigation with NaOCl and Ethylenediaminetetraacetic acid (EDTA) was found to maximize the effectiveness of the antisepsis, due to effective removal of the smear layer and increased dentin permeability [11,12]. Glyde File Prep (Dentsply De Trey GmbH, Germany) that contains hydrogen peroxide [H2O2] and EDTA was recommended to be used with NaOCl in alternating sequence . It is claimed to facilitate endodontic shaping and cleansing due to the chelating EDTA and the effervescence through H2O2. NaOCl/Glyde irrigation procedure may also affect the bond strength to coronal dentin. Beside NaOCl and EDTA effects , residual H2O2 may negatively affect the bond strength . It has been well reported that sodium perborate (SP); a H2O2-releasing agent used intra-coronally for tooth bleaching, reduces the bond strength of resin to coronal dentin . The use of chlorhexidine (CHX) as a ﬁnal rinse was found to enhance the disinfection of the root canal system [9,15]. In addition, encouraging recent studies [16,17] have demonstrated that the application of CHX to dentin decelerated the degradation of the hybrid layer exposed collagen ﬁbrils. CHX was found not to produce detrimental effects to the immediate bond strength [16,17]. However, higher concentrations decreased the bond strength of some adhesive systems . Calcium hydroxide (Ca(OH)2) intracanal dressing was found to increase the healing rate in cases of periradicular lesions  and to promote apexiﬁcation . However, it may be slightly overextended into the pulp chamber during its application with some remnants in contact with coronal dentin. It has been reported that Ca(OH)2 ions diffuse into the smear layer-free dentinal tubules . It was found to decrease the bond strength to root dentin . The purpose of this study was to evaluate the effects of three NaOCl-endodontic irrigation procedures used alone or in combinations with two intermediate dressing materials on shear bond strength of two adhesive composite systems to coronal
S.E. Abo-Hamar dentin. NaOCl or NaOCl–Glyde-File-Prep (H2O2 and EDTA) surface treatments with or without CHX as a ﬁnal rinse were evaluated. Intermediate dressing materials of Ca(OH)2 and SP were also combined with surface treatments for evaluation. Material and methods One-hundred and twenty non-carious human third molars were collected in 0.5% Chloramine solution, cleaned and stored in distilled water (4 C) for a maximum of 6 months . The roots were removed, pulp tissues were removed and pulp chambers were washed with distilled water and ﬁlled with moist cotton pellets in order to avoid drying out of the specimens. Thus, dentin could simulate that of endodontically treated teeth (without intra-pulpal pressure). Then, the crowns were embedded in chemically cured acrylic resin. They were ground ﬂat with a series of SiC-papers ending with 600 grit used on a polisher (Polimet, Buehler) to obtain a 4 mm diameter ﬂat buccal dentin surfaces at 1.5–2.0 mm distance from the pulp (Fig. 1) . Glass rings of 1.5 cm diameter were ﬁxed onto the specimens using ﬂowable composite to create a pulp chamber-like space (Fig. 1). Very thin strings of ﬂowable composite were applied on the outer silane-treated surfaces of the borders of the glass rings. Thus, this ensured that the ﬂowable composite would not contaminate the test area. The chambers could be closed by acrylic covers, which were cemented to the borders of the glass rings using temporary cement (Temp bond NE, Kerr Italia S.p.A., Italy). These closed chambers were intended to keep Ca(OH)2 and SP pastes in place for deﬁned periods and to conﬁne deﬁnite amounts of the irrigants to dentin. The dentin specimens were randomly and equally divided into two main groups (n = 60) and bonded with two adhesive systems/corresponding ﬂowable composite after irrigation procedures: (1) an etch and rinse adhesive system (Excite/Tetric Flow Chroma, [EX/TFC], Vivadent, Liechtenstein) and (2) a self-etching primer system with antibacterial properties (Clearﬁl Protect Bond/Protect Liner F [PB/PLF], Kuraray, Japan) (Table 1). Each group was further subdivided according to the tested endodontic procedures, into 6 groups of 10 specimens each (Fig. 2):
Fig. 1 A diagram showing the model developed to simulate the dentin of pulpless teeth and also the closed pulp chamber. The pulp tissue was excavated and replaced by moist cotton pellet. A glass ring was ﬁxed onto the tooth specimen using ﬂowable composite. The formed chamber was closed by an acrylic cover, which was cemented to the border of the glass ring using temporary cement.
Endodontic materials and bond strength to coronal dentin Table 1
Materials information for bonding procedures.
Excite/Tetric Flow Chroma (EX/TFC), Vivadent
Total Etch: (G07438)a 37% H3PO4b Excite, Primer-adhesive: (G02162) HEMA, DMA, phosphoric acid acrylate, silica, ethanol, initiators
Tetric Flow Chroma: (F53645) Bis-GMA, urethane dimethacrylate and TGDMA (35.0 wt.%). Inorganic ﬁllers (64.6 wt.%). Catalysts, stabilizers and pigments (0.4 wt.%)
Clearﬁl Protect bond/ Protect Liner F (PB/PLF), Kuraray
Primer: (00002A) MDP, HEMA, hydrophilic dimethacrylate, MDPB, ﬂouride, dl-Camphorquinone, N,N-Diethanol-p-toluidine, water) Bond: (00004A) MDP, Bis-GMA, HEMA, hydrophobic dimethacrylate, dlCamphorquinone, N,N-Diethanol-p-toluidine, silanated colloidal silica Clearﬁl Liner Bond2 Protect Liner F: (0056) Bis-GMA, TEGDMA, Silanated colloidal silica, prepolymerized organic ﬁller, ﬂuoride methyl methacrylate, camphorquinone
Batch numbers are in parentheses. Chemical compositions were supplied from the manufacturers’ manuals of products.
Flow chart of the experimental methods. Glyde = Glyde File Prep.
S.E. Abo-Hamar Group 1: Dentin was exposed to distilled water as a control. Group 2: Dentin was exposed to 5.25% NaOCl for 30 min (0.5 ml refreshed every 10 min; simulating the amount clinically in contact with coronal dentin). Group 3: Dentin was exposed three times to: 0.5 ml NaOCl for 5 min, then, 0.5 ml NaOCl mixed with Glyde for 5 min in order to simulate chemo-mechanical root canal instrumentation with NaOCl/Glyde. Then, ﬁnal rinse with NaOCl. Group 4: In addition to chemo-mechanical debridement in group 3 (NaOCl/Glyde), the dentin was washed with saline and 0.5 ml CHX was applied as a ﬁnal rinse (2 min). Saline was used to prevent any interaction between CHX and NaOCl . Group5: In addition to chemo-mechanical debridement (NaOCl/Glyde), Ca(OH)2 was applied for 5 days, removed by excavator and consecutively, dentin was washed with saline, then CHX as a ﬁnal rinse. Group 6: In addition to chemo-mechanical debridement (NaOCl/Glyde), SP paste (mixed with distilled water at 2 g/ml) was applied for 9 days (refreshed every three days), removed and the dentin was washed with saline and then CHX. The compositions of the endodontic materials used are listed in Table 2.
After dentin treatment with the aforementioned protocols, the glass rings were removed and the adhesive systems were applied in standardized circular dentin surfaces of 3 mm in diameter using ﬂat metal rings with 3 mm inner diameter holes and 250 lm height. This ﬂat metal ring assured accurately circular adhesive area without any ﬂashes outside it. Using the Excite system, the dentin surface was acid etched for 15 s, rinsed for 30 s and dried with lint-free absorbent tissue. Then, the primer-adhesive was immediately applied on the dentin circular area with good agitation for 30 s and then gently air dried for 3 s. The primer-adhesive application was repeated in the same manner to ﬁnally obtain a glossy continuous layer and then light cured for 20 s. For the Clearﬁl Protect Bond system, the primer was applied on the dentin for 20 s and then air-thinned with gentle air stream. Then, the adhesive was applied on the dentin circular area with agitation for 20 s. Gentle air stream was applied to obtain a uniform adhesive layer which was light cured for 20 s. Flowable composite rods were built in two increments that were each light cured for 20 s, using a metal ring with a 3 mm diameter hole and 3 mm height. After storage of the specimens in distilled water at 37 C for 24 h, shear bond strength was determined
The medians and the corresponding 25–75% quartiles of the shear bond strength values (MPa) for the groups are shown in Table 3. Results of pairwise comparisons between groups within each composite system and between each other are also shown in Table 3. The application of the Error Rates Method indicated a statistically signiﬁcant inﬂuence of endodontic chemical debridement protocols and adhesive systems in general and irrespective of all other parameters. As shown in Table 3, in comparison to the control group (distilled water) of EX/TFC, NaOCl signiﬁcantly increased the bond strength of EX/TFC (p = 0.009), whereas NaOCl/Glyde and (NaOCl/Glyde)/CHX had no effect. The bond strength to NaOCl/Glyde-treated dentin was signiﬁcantly lower than of NaOCltreated dentin (p = 0.009). On the other hand, when compared to the control group, NaOCl and NaOCl/Glyde had no effect on the bond strength of PB/PLF while (NaOCl/Glyde)/CHX signiﬁcantly decreased this bond strength (p = 0.029). (NaOCl/ Glyde)/Ca(OH)2/CHX signiﬁcantly decreased the bond strength of EX/TFC (p = 0.002) and PB/PLF (p = 0.000). (NaOCl/ Glyde)/SP/CHX signiﬁcantly decreased the bond strength of EX/TFC (p = 0.000) and PB/PLF (p = 0.000). Discussion In the experimental design of the present study, the clinically applied irrigation and dressing procedures were simulated in groups, rather than separate endodontic materials that would obtain more clinically signiﬁcant results. Studies investigated the effect of endodontic irrigants are sufﬁcient [4–7,18], whereas those investigated endodontic irrigants in combinations are scarce [3,8]. The NaOCl/Glyde irrigation protocol
Chemical compositiona b
Hypochlorite SPEIKO [SPEIKO-Dr. Speier GmbH, Germany] Glyde File Prep [Dentsply De Trey GmbH, Konstanz, Germany] Chlorhexidine [Sigma Chemicals Co., St. Louis, MO, USA] Hypocal SN [Merz Dental GmbH, Germany] Sodium perborate Bleaching agent [Merck, Darmstadt, Germany] a
Materials information for endodontic procedures.
using a Material Testing Machine (Zwick 010, Ulm, Germany) at a cross head speed of 0.75 mm/min . A chisel-shaped rod was placed at a distance of 70 lm from and parallel to the adhesive interface . Medians and 25–75% quartiles were determined from ten specimens of each experimental group, and pairwise comparisons between groups were performed using the Mann–Whitney-Wilcoxon rank sum test (PC+, version 15, SPSS, Chicago, III., USA) at the 0.05 level of signiﬁcance (a). The Error Rates Method was applied to detect signiﬁcant differences between endodontic procedures and between adhesive systems in general by adjusting a to a\ = 1 (1 a)1/K (K = number of performed pairwise tests).
5.25% NaOCl Ethylenediametetracetic acid (EDTA) and carbamide peroxide in water soluble base 0.2% Chlorhexidine digluconate 100 g paste contain: 45 g Calcium hydroxide and 5 g Barium sulfate Sodium perborate trihydrate
Chemical compositions were supplied from the manufacturers’ manuals of products. Manufacturers of materials are in brackets.
Endodontic materials and bond strength to coronal dentin Table 3
Dentin shear bond strengths for different endodontic procedures.
Experimental groups (n = 10)
Median bond strength values (25–75% quartiles) of EX/TFC
(1) (2) (3) (4) (5) (6)
21 26 21 22 17 14
Distilled water NaOCl NaOCl/Glyde NaOCl/Glyde + CHX NaOCl/Glyde + Ca(OH)2 + CHX NaOCl/Glyde + Na perborate + CHX
(20, (24, (18, (20, (15, (13,
24)A *,a# 26)A,b 23)A,a 27)A,ab 18)B,c 15)D,d
Median bond strength values (25–75% quartiles) of PB/PLF 18 18 17 16 11 11
(17, 18)B,a (16, 19)B,ab (13, 19)BD,ab (14, 17)BD,b (9, 14)D,c (11, 13)C,c
Signiﬁcant differences between the two composite systems are indicated by different capital letters. Signiﬁcant differences between groups within each composite system are indicated by different small letters.
may be optimal especially in cases of necrotic pulp with infected dentinal tubules . The addition of CHX as a ﬁnal rinse may be more prognostic in these cases .The use of NaOCl-alone irrigation protocol may be satisfactory in simple cases of vital pulp with irreversible pulpitis . For testing the bond strength, buccal dentin surfaces were used to standardize the substrate as much as possible and as required by ISO-standard No. 11405 (2003) . This reduces variation of data and enables studying the effect of endodontic irrigation protocols. Shear bond strength test was meticulously performed. 0.75 mm/min cross head speed was used as recommended in literature . Due to the non-uniform stress distribution at the interface, the offset distance (distance from the dentin surface to the point of load application) was minimized to be 70 lm. This minimizes stress concentration inside the dentin substrate leading to less cohesive failure in dentin . In the present study; partial cohesive failure in dentin did not exceed 30% of the specimens per group and the coefﬁcient of variation ranged from 10% to 26% in all groups. In contrast, in the microtensile bond strength (lTBS) test (non-trimming technique), the stress distribution across the adhesive interface is uniform, however the tensile forces are applied on the adhesive interface passing through the two adherents resulting in some cohesive failure either in composite or in dentin . In addition, producing mini-sticks requires cutting using slow speed saw that may either slightly decrease the bond strength or lead to premature failure of originally low bond strength specimens . Previously, it was found that 5% NaOCl application to dentin for 60 min caused 80–100 lm dentin subsurface deproteinization . It appeared as pores that were originally occupied by collagen ﬁbers . In the NaOCl groups of the present study, 5.25% NaOCl was applied on dentin for 30 min (refreshed every 10 min). The subsequent demineralization by the phosphoric acid of Excite and the primer of Protect Bond that was found to be 12 lm  and 0.5 lm , respectively, may result in a dentin subsurface deproteinized layer. It may be inﬁltrated by resin to a certain depth forming what is called a reverse hybrid layer . This exposed collagen-free hybrid layer might positively affect the bond strength [31,34]. Besides, the previously reported NaOCl negative oxidizing effect on the bond strength [4,5] was found not to essentially affect all the adhesive systems . The results of the present study showed that NaOCl-alone irrigation procedure signiﬁcantly increased the bond strength using EX/TFC, whereas it did not signiﬁcantly affect the bond strength using PB/PLF. In the literature, the lTBS of Excite to
dentin was not affected by 10 min of 5% NaOCl , which indicated that NaOCl has little or no negative oxidizing effect on Excite. Therefore, in the present study, the longer NaOCl application period with increased deproteinization depth, may explain the increased bond strength. On the other hand, it was found in literature that the lTBS of Clearﬁl Protect Bond to dentin was signiﬁcantly reduced by 30 s of 6% NaOCl; however, the use of reducing agents (5 or 10 s of accel or rosmarinic acid) successfully recovered it . In the present study, the longer NaOCl application period may also explain the stable bond strength of PB/PLF. It should be mentioned that short NaOCl application periods [4,5] do not simulate the clinical irrigation period. Another study that used 1% NaOCl (refreshed every 5 min) for long period (1 h), increased the lTBS of a self etching adhesive system (XENO III, Dentsply) to dentin . In NaOCl/Glyde groups of the present study, NaOCl and NaOCl–Glyde (EDTA + H2O2) were alternately applied on dentin three times (each for 5 min). It has been reported that the combined use of NaOCl and EDTA leads to interaction between them causing NaOCl to lose its tissue-dissolving capacity, whereas EDTA retained its calcium-chelating ability during the ﬁrst 7 min of the reaction . Therefore, in the present study, the alternating deproteinizing NaOCl and decalcifying EDTA may erode the coronal dentin surface  resulting, after application of the adhesive systems, in an almost normal hybrid layer. This may explain the results of the present study that showed that the bond strength of EX/TFC in NaOCl/Glyde group was signiﬁcantly lower than NaOCl group but was in the range of the control group. The retention of H2O2 to dentin might be too low to affect the bond strength. On the other hand, the bond strength of PB/PLF in NaOCl/Glyde group was not signiﬁcantly lower than the NaOCl- or the distilled water groups. However, the relatively high coefﬁcient of variation (20%) of NaOCl/Glyde group, and the signiﬁcant decrease of the bond strength of (NaOCl/Glyde)/CHX group in comparison to the distilled water group, may indicate the possible NaOCl and/or H2O2 negative effects on the bond strength of PB/PLF. To date, no study has evaluated the effect of NaOCl/ Glyde irrigation protocol on the bond strength to dentin. In the literature, 5.25% NaOCl for 5 min (refreshed every 1 min) followed by EDTA for 1 min resulted in a signiﬁcant decrease of the lTBS of Clearﬁl SE Bond, Kuraray (self-etching primer system), whereas it did not affect that of XPBond, Dentsply (etch and rinse system) . In the present study, no signiﬁcant difference was found between (NaOCl/Glyde)/CHX and NaOCl/Glyde groups. Thus,
66 the addition of CHX to NaOCl/Glyde irrigation procedure did not affect the bond strength of each adhesive system and this is in line with the literatures [16,17]. The signiﬁcant decrease of the PB/PLF bond strength in (NaOCl/Glyde)/CHX group in comparison to distilled water group does not necessarily due to the contribution of 0.2% CHX. It has been reported that CHX may reduce the lTBS of some self-etch adhesives, due to a possible interaction between them. However, this was true at 2% concentration and not for 0.12% concentration . The results of the present study showed that addition of Ca(OH)2 for 5 days to the (NaOCl/Glyde)/CHX group signiﬁcantly decreased the bond strength using either EX/TFC or PB/ PLF. This is in line with previous ﬁndings [22,23]. Partial obliteration of the dentinal tubules by Ca(OH)2 might act against proper etching and inﬁltration of adhesive resin into the dentinal tubules. In the present study, Ca(OH)2 dressing decreased the bond strength of EX/TFC by 23%, which was less than the decrease observed with PB/PLF (31%). This may be explained by the phosphoric acid of EX/TFC that could decalcify larger thickness of the dentin surface when compared to the effect of the self-etching primer of PB/PLF, removing the highest concentration of the Ca(OH)2 powder diffused inside the dentinal tubules. It may be suggested that if Ca(OH)2 was inadvertently left in the coronal part, it should be carefully excavated. EDTA solution, which was recommended be used to eliminate the Ca(OH)2 dressing from the root canal, may also be used during its excavation from the coronal part. Also, delaying of the immediate restoration with a wet cotton pellet inside the access cavity under a temporary ﬁlling might allow Ca(OH)2 to diffuse out of the dentinal tubules. The negative oxidizing effect of SP was conﬁrmed in the present study. The addition of SP to (NaOCl/Glyde)/CHX group signiﬁcantly decreased the bond strengths of both the adhesive systems and this in line with literature . This may be explained by residuals of the oxygen forced inside the dentinal tubules during the long intracoronal bleaching period (9 days). Oxygen residuals may inhibit resin polymerization and also interfere with the resin inﬁltration . Delaying of the restoration of the bleached tooth for two weeks was found to recover this reduced bond strength . Conclusions Based on the results of the present study, EX/TFC may be used within the pulp chamber after NaOCl-alone, NaOCl– Glyde-File-Prep or NaOCl–Glyde-File-Prep–CHX irrigation regimens tested in the present study. For PB/PLF, further investigations are needed to test if the application of a reducing agent after the irrigation procedure would be sufﬁcient to obtain optimal bond strength. Ca(OH)2 intermediate dressing should not be overextended into the pulp chamber. New methods for optimal removal of Ca(OH)2 should be studied in order to enhance the bond strength after Ca(OH)2 use. Acknowledgements I wish to express my thanks and appreciation to Dr. KarlAnton Hiller, PhD, mathematician, Department of Operative Dentistry and Periodontology, University of Regensburg,
S.E. Abo-Hamar Germany, for his excellent performance of the statistics of this research. I also wish to express my thanks and appreciation to Prof. Dr. Stephen C. Bayne, Michigan University., US, for his constructive criticism and for his advice concerning the manuscript. References  Gillen BM, Looney SW, Gu LS, Loushine BA, Weller RN, Loushine RJ, Pashley DH, Tay FR. Impact of the quality of coronal restoration versus the quality of root canal ﬁllings on success of root canal treatment: a systematic review and metaanalysis. J Endod 2011;37:895–902.  Schwartz RS, Fransman R. Adhesive dentistry and endodontics: materials, clinical strategies and procedures for restoration of access cavities: a review. J Endod 2005;31:151–65.  Yurdagu¨ven H, Tanalp J, Toydemir B, Mohseni K, Soyman M, Bayirli G. The effect of endodontic irrigants on the microtensile bond strength of dentine adhesives. J Endod 2009;35:1259–63.  Prasansuttiporn T, Nakajima M, Kunawarote S, Foxton RM, Tagami J. Effect of reducing agents on bond strength to NaOCltreated dentin. Dent Mater 2011;27:229–34.  Lai SC, Mak YF, Cheung GS, Osorio R, Toledano M, Carvalho RM, Tay FR, Pashley DH. Reversal of compromised bonding to oxidized etched dentin. J Dent Res 2001;80:1919–24.  Ozturk B, Ozer F. Effect of NaOCl on bond strength of bonding agents to pulp chamber lateral walls. J Endod 2004;30:362–5.  Giovannone T, Migliau G, Bedini R, Ferrari M, Gallottini L. Bond strength to deep coronal dentin: effect of bonding strategies. Minerva Stomatol 2007;56:105–14.  Cecchin D, Farina AP, Galafassi D, Barbizam JV, Corona SA, Carlini-Ju´nior B. Inﬂuence of sodium hypochlorite and edta on the microtensile bond strength of a self-etching adhesive system. J Appl Oral Sci 2010;18:385–9.  Sena NT, Gomes BP, Vianna ME, Berber VB, Zaia AA, Ferraz CC, Souza-Filho FJ. In vitro antimicrobial activity of sodium hypochlorite and chlorhexidine against selected single-species bioﬁlms. Inter Endod J 2006;39:878–85.  Marending M, Luder HU, Brunner TJ, Knecht S, Stark WJ, Zehnder M. Effect of sodium hypochlorite on human root dentine – mechanical, chemical and structural evaluation. Inter Endod J 2007;40:786–93.  Soares JA, Roque de Carvalho MA, Cunha Santos SM, Mendonc¸a RM, Ribeiro-Sobrinho AP, Brito-Ju´nior M, Magalha˜es PP, Santos MH, de Maceˆdo Farias L. Effectiveness of chemomechanical preparation with alternating use of sodium hypochlorite and EDTA in eliminating intracanal Enterococcus faecalis bioﬁlm. J Endod 2010;36:894–8.  Lim TS, Wee TY, Choi MY, Koh WC, Sae-Lim V. Light and scanning electron microscopic evaluation of Glyde File Prep in smear layer removal. Inter Endod 2003;36:336–43.  Grande NM, Plotino G, Falanga A, Pomponi M, Somma F. Interaction between EDTA and sodium hypochlorite: a nuclear magnetic resonance analysis. J Endod 2006;32:460–4.  Attin T, Paque F, Ajam F, Lennon AM. Review of the current status of tooth whitening with the walking bleach technique. Inter Endod J 2003;36:313–29.  Zamany A, Safavi K, Spangberg LS. The effect of chlorhexidine as an endodontic disinfectant. Oral Surg Oral Med Oral Pathol Oral Radiol Endod 2003;96:578–81.  Ricci HA, Sanabe ME, de Souza Costa CA, Hebling J. Chlorhexidine increases the longevity of in vivo resin–dentin bonds. Eur J Oral Sci 2010;118:411–6.  Loguercio AD, Stanislawczuk R, Polli LG, Costa JA, Michel MD, Reis A. Inﬂuence of chlorhexidine digluconate
Endodontic materials and bond strength to coronal dentin
concentration and application time on resin–dentin bond strength durability. Eur J Oral Sci 2009;117:587–96. Campos EA, Correr GM, Leonardi DP, Pizzatto E, Morais EC. Inﬂuence of chlorhexidine concentration on microtensile bond strength of contemporary adhesive systems. Braz Oral Res 2009;23:340–5. Trope M, Delano EO, Ørstavik D. Endodontic treatment of teeth with apical periodontitis: single vs. multivisit treatment. J Endod 1999;25:345–50. Shabahang S, Torabinejad M, Boyne PP, Abedi H, McMillan P. A comparative study of root-end induction using osteogenic protein-1, calcium hydroxide, and mineral trioxide aggregate in dogs. J Endod 1999;25:1–5. Foster KH, Kulild JC, Weller RN. Effect of smear layer removal on the diffusion of calcium hydroxide through radicular dentin. J Endod 1993;19:136–40. Barbizam JV, Trope M, Teixeira EC, Tanomaru-Filho M, Teixeira FB. Effect of calcium hydroxide intracanal dressing on the bond strength of a resin-based endodontic sealer. Braz Dent J 2008;19:224–7. ISO (International Organization for Speciﬁcations): ISO/TS 11405, Dental Materials-Testing of adhesion to tooth structure; 2003. Roberts S, Kim JR, Gu LS, Kim YK, Mitchell QM, Pashley DH, Tay FR. The efﬁcacy of different sealer removal protocols on bonding of self-etching adhesives to AH plus-contaminated dentin. J Endod 2009;35:563–7. Krishnamurthy S, Sudhakaran S. Evaluation and prevention of the precipitate formed on interaction between sodium hypochlorite and chlorhexidine. J Endod 2010;36:1154–7. Hara AT, Pimenta LA, Rodrigues Jr AL. Inﬂuence of crosshead speed on resin-dentin shear bond strength. Dent Mater 2001;17:165–9.
67  Versluis A, Tantbirojn D, Douglas WH. Why do shear bond tests pull out dentin? J Dent Res 1997;76:1298–307.  Villegas JC, Yoshioka T, Kobayashi C, Suda H. Obturation of accessory canals after four different ﬁnal irrigation regimes. J Endod 2002;28:534–6.  Scherrer SS, Cesar PF, Swain MV. Direct comparison of the bond strength results of the different test methods: a critical literature review. Dent Mater 2010;26:78–93.  Abreu CW, Santosb JF, Passos SP, Michida SM, Takahashi FE, Bottino MA. The inﬂuence of cutting speed and cutting initiation location in specimen preparation for the microtensile bond strength test. J Adhes Dent 2011;13:221–6.  Prati C, Chersoni S, Pashley DH. Effect of removal of surface collagen ﬁbrils on resin-dentin bonding. Dent Mater 1999;15:231–323.  Santini A, Miletic V. Quantitative micro-Raman assessment of dentine demineralization, adhesive penetration, and degree of conversion of three dentine bonding systems. Eur J Oral Sci 2008;116:177–83.  Sidhu SK, Omata Y, Tanaka T, Koshiro K, Spreaﬁco D, Semeraro S, Mezzanzanica D, Sano H. Bonding characteristics of newly developed all-in-one adhesives. J Biomed Mater Res B Appl Biomater 2007;80:297–303.  Sauro S, Mannocci F, Toledano M, Osorio R, Pashley DH, Watson TF. EDTA or H3PO4/NaOCl dentine treatments may increase hybrid layers’ resistance to degradation: a microtensile bond strength and confocal-micropermeability study. J Dent 2009;37:279–88.  Zhang K, Tay FR, Kim YK, Mitchell JK, Kim JR, Carrilho M, et al.. The effect of initial irrigation with two different sodium hypochlorite concentrations on the erosion of instrumented radicular dentin. Dent Mater 2010;26:514–23.